advertisement

Experimental and physics-based modeling assessment of strain induced mobility enhancement in FinFETs N. Serra1 , F. Conzatti1 , D. Esseni1 , M. De Michielis1 , P. Palestri1 , L. Selmi1 , S. Thomas2 , T.E. Whall2 , E.H.C. Parker2 , D.R. Leadley2 , L. Witters3 , A. Hikavyy3 , M.J. Hÿtch4 , F. Houdellier4 , E. Snoeck4 , T.J. Wang5 , W.C. Lee5 , G. Vellianitis6 , M.J.H. van Dal6 , B. Duriez6 , G. Doornbos6 and R.J.P. Lander6 1 DIEGM, Via delle Scienze 208, 33100 Udine, Italy, 2 University of Warwick, UK, 3 IMEC, Belgium, 4 CEMES-CNRS, France, 5 TSMC, Hsinchu, Taiwan, 6 NXP-TSMC Research Center, Leuven, Belgium. e.mail: nicola.serra@uniud.it Abstract This study combines direct measurements of channel strain, electrical mobility measurements and a rigorous modeling approach to provide insight about the strain induced mobility enhancement in FinFETs and guidelines for the device optimization. Good agreement between simulated and measured mobility is obtained using strain components measured directly at device level by a novel technique. A large vertical compressive strain is observed in FinFETs and the simulations show that this helps recover the electron mobility disadvantage of the (110) FinFETs lateral interfaces w.r.t. (100) interfaces, with no degradation of the hole mobility. The model is then used to systematically explore the impact of the ﬁn-width, ﬁnheight and ﬁn-length stress components on n- and p-FinFETs mobility and to identify optimal stress conﬁgurations. Introduction FinFETs enable scaling of CMOS by enhancing electrostatic control [1, 2, 3], and strain is an important technology booster [3, 4, 5]. Strain induced mobility enhancement in planar MOSFETs has been studied extensively [6, 7, 8, 9], but the complex stress conﬁgurations in FinFETs, consisting of TfL , TfH and TfW components (see Fig.1), still demand physicsbased models to support device design. In fact, so far the stress conﬁgurations in FinFETs have been typically inferred from process simulations and the analysis of mobility data has been based on the piezo-resistive coefﬁcients [3, 4, 10], that offer limited insight and are inaccurate at high stress [11] and for complex stress conﬁgurations as in Fig.1. Furthermore, for narrow ﬁns, mobility data is limited and strain measurement is challenging for established techniques [12, 13]. This paper presents an assessment of the strain induced mobility enhancement based on direct strain measurements, electrical mobility measurements and numerical physics-based modeling. Mobilities in narrow n- and p-FinFETs, measured from 77K to 300K, are compared with a state-of-the-art transport model based on the Boltzmann Transport Equation (BTE) in inversion layers, accounting for all the relevant scattering mechanisms, in which strain is implicitly introduced by modiﬁcation of the band structure. Simulations are then used to 97-4244-5640-6/09/$26.00 ©2009 IEEE clarify the physical mechanisms for mobility enhancement and to provide guidelines for the device optimization. Device fabrication and characterization 22nm node FinFETs were fabricated using a VLSI-compatible process [1, 2] (Fig.2). Strain components εzz , εyy (z, y being the ﬁn-height and ﬁn-width directions, see DCS in Fig.1) of fully-processed devices were quantiﬁed directly by holographic interferometry [14, 15] (Figs.3 and 4). This novel technique is capable of measuring strain with nanometer spatial resolution and for relatively thick samples, thus suppressing the inﬂuence of sample relaxation. Measured εzz is very large, especially w.r.t. the low intrinsic stress of the TiN (Fig.5(a)), but it is consistent with strain induced by differences in thermal expansion coefﬁcients following plastic relaxation at high temperature (Fig.5(b)). Mobility was extracted in 10μm long, 65nm tall FinFET devices consisting of 10 ﬁns in parallel by split C−V and I−V measurements. The drain current was measured at VDS =10mV and corrected for gate leakage current, while the inversion charge Ninv was obtained by integration of the gateto-channel capacitance curve; the channel area was obtained as 10·Lﬁn ·(2Hﬁn + Wﬁn ). Due to excessive gate leakage current, at Ninv larger than approximately 2 · 1013 cm−2 the extracted mobility data were not considered to be reliable. Figs.6 and 7 compare the electron and hole mobility to literature data. Electron mobility is signiﬁcantly larger than for planar MOSFETs in the Ninv range of interest (≥2·1012 cm−2 ). At low Ninv values the measured mobility shows a clear roll-off, stronger than in the reference data, most likely due to scattering by Coulomb centers in the high-κ stack [16]. Hole mobility is comparable to literature data [17, 18, 20]. Mobility model and validation The transport analysis is focussed on the lateral (110)/110 interfaces of the FinFETs simulated as double-gate devices. For a ﬁn height of 65nm this assumption is appropriate for ﬁn widths below approximately 20nm. The n-type devices were simulated with the Multi Subband Monte Carlo (MSMC) approach that accounts for the subband quantization and for the 4.2.1 IEDM09-71 most important scattering mechanisms [22]. Fig.8 shows a sketch of the Δ4 and the Δ2 valleys in a (110)/[110] electron inversion layer. In unstrained devices the Δ4 valleys are the lowest due the largest quantization mass my =0.315m0 . It has been argued that, due to the non parabolicity of the Δ silicon valleys in the [110] direction, the parabolic effective mass approximation (EMA) is inaccurate for the Δ2 valleys in (110) inversion layers [24]. We used a quantization model based on the Linear Combination of Bulk Bands (LCBB [25]) to extract a modiﬁed quantization mass my,eﬀ =0.23m0 for the Δ2 valleys, yielding good agreement of the EMA and the LCBB results [26]. Hole mobility was calculated starting from the band-structure obtained with a self-consistent k·p solver coupled to the Poisson equation (as in [6, 7]), and then by using the momentum relaxation time approximation and accounting for phonons and surface roughness scattering by following [6]. All the scattering rates were calculated by using, for each subband, the envelope wave-function corresponding to k=0 [6]. The scattering parameters of Tab.1 were used for all the simulations of this paper. Figs.9 and 10 show good agreement between simulations and experiments for unstrained MOSFETs. The strain modeling starts by converting the TfH , TfW , TfL stress components in the DCS to the corresponding strain tensor εc in the CCS (see Fig.1), by using appropriate rotation matrices and the silicon elastic compliance tensor. Then for electrons we calculated, for each strain tensor εc , the Δ4 and the Δ2 valley splitting and modulation of the effective masses using the results of [27], derived from a two band k·p approach and validated against pseudo-potential calculations. These values were directly used in the MSMC simulations. For holes, instead, the εc enters directly the matrix of the k·p calculations [6], hence the band-structure and the mobility determination; Fig.11 shows the strong deformation of the hole band-structure produced by the uniaxial stress. Figs.12, 13 show good agreement between simulations and experiments obtained for uniaxially strained (110)/110 planar devices. Mobility in strained FinFETs Mobility variations versus TfL , TfH and TfW are plotted in Figs.14, 15. Although qualitatively consistent, the piezoresistive model yields large quantitative discrepancies w.r.t. the numerical simulations. Consistently with Figs.12, 13, tensile and compressive TfL enhances electron and hole mobility, respectively. Furthermore a compressive TfH increases the electron mobility, while it hardly affects hole mobility (see Tab.2). To quantitatively investigate the effect of TfH , Figs.16, 17 show that the mobility simulations obtained by using the measured strain values of Fig.4 are in fairly good agreement with measured data; in this respect, the DCS strain conﬁguration of Figs.4 (εzz =−0.8% and εyy =+0.3%) corresponds to a dominant TfH stress component of approximately -1.1GPa. As for the interpretation of the electron mobility enhancements with compressive TfH , Fig.8 shows that the Δ2 valleys have a IEDM09-72 smaller transport mass mx than the Δ4 valleys. Compressive TfH yields a negative Δ2 to Δ4 valley splitting that improves the mobility through the re-population of the Δ2 subbands (see Fig.18). Figs.19 and 20 investigate the additivity of the TfL , TfW and TfH effects for mobility optimization. A tensile TfL further improves electron mobility w.r.t. the values obtained with compressive TfH , while a compressive TfL increases the hole mobility. Fig.20 shows that the TfW is not as effective as the TfL for device optimization. Fig.19 and Fig.20 show that the piezo-resistive model results in quantitative and even qualitative discrepancies w.r.t. the numerical simulations and underlines the need for a rigorous modeling approach. Finally, the additive effect of different strain components is experimentally conﬁrmed by the stress induced IDS improvements reported in Fig.21 for nano-scale FinFETs. Conclusions In summary, direct strain measurements, mobility characterization and physics-based modeling were used to explain and optimize strain in both n- and p-type FinFETs. Our results assessed and explained the potentials for large electron mobility enhancements produced by the vertical strain and discussed the impact of all the main strain components on the electrical mobility. All the main simulation predictions were conﬁrmed by experiments. Acknowledgments Work partially funded by the EU “NANOSIL NoE (FP7 IST-216171)”. References [1] M.J.H. van Dal et al. in VLSI, pp.110, 2007 [2] G. Vellianitis et al. in IEDM, pp.681, 2007 [3] S. Suthram et al. in IEEE EDL, pp.480, 2008 [4] K-M. Tan et al. in IEEE EDL, pp. 769, 2006 [5] T-Y. Liow et al. in IEEE TED, pp. 2475, 2008 [6] M.V. Fischetti et al. in JAP, pp.1079, 2003 [7] T. Krishnamohan et al. in IEDM, pp.899, 2008 [8] Y. Zhao et al. in IEDM, pp.577, 2008 [9] M. Saitoh et al. in IEDM, pp.573, 2008 [10] M. Saitoh et al. in VLSI, pp.18, 2008 [11] A.T. Pham et al. in ULIS Conf. Proc., pp.121, 2009 [12] P. Zhang et al. in APL, 89, pp. 161907, 2006 [13] J. Li et al. in APL, 87, pp. 222111, 2005 [14] M.J. Hÿtch et al. in Nature, 453, pp. 1086, 2008 [15] M.J. Hÿtch et al. Patent Application PCT N PCT/FR2008/001302 [16] P. Toniutti et al. in ESSDERC Conf. Proc., 2008 [17] H. Irie et al. in IEDM, pp.225, 2004 [18] W. Xiong et al. in Dev. Res. Conf., pp.39, 2006 [19] S. Takagi et al. in IEEE TED, pp.2363, 1994 [20] G. Tsutsui et al. in IEEE TED, pp.2582, 2006 [21] S. Takagi et al. in IEEE TED, pp.2357, 1994 [22] L. Lucci et al. in IEEE TED, pp.1156, 2007 [23] C. Jacoboni et al. in Rev.Mod.Phys., pp.645, 1983 [24] K. Uchida et al., in IEDM, pp.1019, 2006 [25] D. Esseni et al. in Phys. Rev.B, pp. 165342, 2005 [26] N. Serra et al. in ULIS Conf. Proc., pp.113, 2009 [27] E. Ungersboeck et al., IEEE TED, pp.2183, 2007 [28] C.S. Smith et al. in Phys. Rev-, vol.94, pp.42, 1954 4.2.2 Figure 1: Schematic of a FinFET indicating the stress components in the ﬁn height TfH , width TfW and length TfL direction in the Device Coordinate System (DCS). Complex stress conﬁgurations comprising several TfH , TfW and TfL components may occur in the device. Also shown is the silicon Crystal Coordinate System (CCS). Figure 2: Cross-section TEM image through the gate-plane of FinFETs with Wﬁn =20nm Figure 5: Maximum vertical strain εzz,Si in interferometry of deformation in vertical direction, εzz , calculated from (004) fringes for 20nm wide ﬁns (as pictured in Fig.2). (b) vertical (Hﬁn ) directions, calculated respectively from (111) and (111) holographic fringes for 10nm wide ﬁns. 300 (110)/[110] 15 This work, n-FinFET TSi 16 to 36nm -3 NA=2.8x10 cm This work, p-FinFET TSi 16 and 26nm holes 200 100 electrons 2 2 700 600 500 400 Carrier mobility [cm /Vs] Figure 4: Deformation in (a) lateral (Wﬁn ) and Carrier mobility [cm /Vs] Figure 3: Direct measurement by holographic Planar p-MOS [17] 15 -3 p-FinFET (NA=2x10 cm ) [18] Planar (110) n-MOS [19] DG p-MOS TSi=32nm [20] 300K This work,n-FinFETs TSi=16 to 36nm (110)/[110] 1000 15 11 12 10 10 -2 10 Inversion layer density [cm ] This work, p-FinFETs TSi=16 and 36nm Planar n-MOSFET 77K [19] 13 Figure 6: Measured electron and hole mobility at 300K for the n- and p-FinFETs of this work, compared to literature data for planar MOSFETs [17, 19, 20] or FinFETs [18]. All devices have very low channel doping concentrations below 5x1015 cm−3 . Surface Roughness: Holes Electrons (Exp. spectrum) Δ[nm] 0.24 0.9 Lc [nm] 4 1.2 Phonons: Holes Electrons Acoustic Dacc [eV] 10.2 13 Optical Dopt [108 eV/cm] 15 from [23] Optical Ph. Energy [meV] 62 from [23] -3 NA=2.8x10 cm 100 12 Si ﬁn (a) post-TiN deposition and (b) after thermal cycle. As-deposited strain is due to intrinsic stress in TiN and, for post-thermal cycle, to plastic relaxation at high temperature. CTE is the coefﬁcient of thermal expansion and E is Young’s modulus. Wﬁn =16nm and TTiN =7nm. 77K 13 10 10 -2 Inversion layer density [cm ] Table 1: Scattering parameters used in all sim- Figure 7: Measured electron and hole mobility at 77K for the n- and p-FinFETs of this work, compared to literature data for planar MOSFETs [19]. All devices have very low channel doping concentrations below 5x1015 cm−3 . ulations. Electron optical phonons model from [23]. Screening is not accounted for in the hole mobility calculations, hence the Lc is relatively large to reproduce the measured mobility vs. Feﬀ slope at large Feﬀ (see Fig.10). Figure 8: Δ4 and Δ2 valleys for the elec- trons in a (110)/[110] Si inversion layer. Mobility enhancements are obtained when stress forces the re-population of the Δ2 valleys with the lowest mass mx in the transport direction (see Fig.1). my is the quantization mass that enters the Schrödinger equation. (110)/[110] Si 15 NA=3.9x10 cm 15 NA=2.8x10 cm 133K -3 3 -3 300K 100 Lines: Experiments [19] Symbols: Simulations 0.1 1 Feff [MV/cm] Figure 9: Simulated and experimental electron mobility (unstrained) versus effective ﬁeld in (110) inversion layers, at 300K and 133K. Measurements from [19]. 4.2.3 Lines: Experiments Symbols: Simulations 10 77K (a) 2 1000 Hole mobility [cm /Vs] 2 Electron mobility [cm /Vs] 3 10 (b) (110)/[110] 223K 2 10 (110)/[001] 300K 2 (001) 0.1 Feff [MV/cm] (110) 1.0 10 12 10 300K 10 13 -2 Pinv [cm ] Figure 10: Simulated and experimental hole mobility (unstrained): (a) versus the effective ﬁeld Feﬀ in (001) Si (for different temperatures); (b) versus the inversion density in (110) Si. Measurements from [21] (a), [17] (b). IEDM09-73 10 [001] unstr. -1.5GPa [110] +1.5GPa [110] [110] [110] stress 0 [001] stress -5 12 Pinv=8x10 cm (110)/[110] n-MOS 12 -2 Ninv=5x10 cm Figure 11: Hole equi-energy contour plots for the lowest subband at 100meV from the subband minimum for unstrained or strained (110) inversion layer. 100 -50 Δμ/μ [%] TfW 12 -1 Figure 13: Simulations and measurements [17] of hole mobility variations in uniaxially strained (110)/110 bulk planar p-MOSFETs. TfH TfL TfW 12 -100 -2 1.5 -1.5 -1 -0.5 0 0.5 1 Stress level [GPa] 1.5 Figure 15: Simulated stress induced hole mobility variations vs. TfH , TfL , TfW at Pinv =8x1012 cm−2 in (110) Si. Results are also shown for piezo-resistive model with the bulk Si coefﬁcients [28]. Table 2: Table summarizing the impact of different stress components on the electron and hole (110)/[110] FinFETs mobility. (EΔ2-EΔ4) = 92.25x10 300K -3 Experiments [19] Measured TSi=16nm 300K Measured TSi=16nm 77K Sim. Unstrained 300K Sim. εzz=-0.8% εyy=+0.3% 300K Sim. εzz=-0.8% εyy=+0.3% 77K 100 11 10 12 (110)/[110] p-FinFET 1000 77K 2 2 77K Relative occupation [%] (110)/[110] n-FinFET Hole mobility [cm /Vs] Electron mobility [cm /Vs] 0 15 300K Measured TSi=16nm 300K Measured TSi=16nm 77K Sim. Unstrained 300K Sim. εzz=-0.8% εyy=+0.3% 300K 100 Sim. εzz=-0.8% εyy=+0.3% 77K 13 12 10 10 -2 Ninv (single gate) [cm ] 13 10 holes Δμ/μ [%] 100 60 12 Ninv=8x10 cm -2 40 20 0 -0.5 -1.0 -1.5 -2.0 Fin-height stress TfH [GPa] valleys in (110)/[110] n-FinFET vs. compressive TfH (bottom x-axis). The top x-axis shows the stress induced Δ2 to Δ4 valley splitting that concurs with the quantization to the overall subbands splitting. electrons solid+symb.: simulations dashed: piezoresistive model 0 TfL [GPa] 2 0 holes Figure 19: Simulated stress induced electron and hole mobility (a), and corresponding percentage mobility variations w.r.t. the unstrained case (b) vs. TfL and for TfH =-1GPa. -2 1400 600 electrons TfH= -1GPa -1 0 TfW [GPa] 1 2 Figure 20: Simulated stress induced electron and hole percentage mobility variations w.r.t. the unstrained case vs. TfW and for TfH =-1GPa. 4.2.4 400 pMOS nMOS 1200 15nm = Wfin = 13nm 57nm = LG = 45nm 300 0 -1.0 800 400 VDS=±1V Hfin=65nm -0.5 1000 600 dashed: unstrained solid: strained 200 100 solid+symb.: simulations dashed: piezoresistive model -100 (b) 1 -2 500 -50 holes -1 12 Ninv= 8x10 cm 50 (a) -2 50 IEDM09-74 -0.2 Figure 18: Simulated re-population of the Δ2 ID,sat [μA/μm] 12 Ninv= 8x10 cm TfH= -1GPa Δμ/μ [%] 2 μ [cm /Vs] 100 300 -50 -2 TfH [eV] -0.15 electrons 400 0 -0.1 Δ4 valleys 0.0 Figure 17: Measured and simulated hole mobility in p-FinFETs at 300K and 77K. Strain values εzz =−0.8% and εyy =+0.3% taken from Figs.4. -0.05 -12 Δ2 valleys 80 -2 500 100 100 10 Pinv (single gate) [cm ] Figure 16: Measured and simulated electron mobility in n-FinFETs at 300K and 77K. Strain values εzz =−0.8% and εyy =+0.3% taken from Figs.4. 200 100 Holes, Pinv= 8x10 cm -0.5 0 0.5 1 Stress level [GPa] NA=2.8x10 cm 80 0 -50 -2 Figure 14: Simulated stress induced electron mobility variations vs. TfH , TfL , TfW at Ninv =8x1012 cm−2 in (110) Si. Results are also shown for the piezo-resistive model with the bulk Si coefﬁcients [28]. 1000 40 60 Stress [MPa] Dashed: piezoresistive model Solid+Symb.: Simulations Electrons, Ninv= 8x10 cm -1.5 20 50 TfH 0 (110)/[110] p-MOS 13 -2 Pinv=1x10 cm 0 0.05 0.1 Tensile Strain (%) 100 TfL [110] tens. stress -4 Figure 12: Simulations and measurements [24] of electron mobility variations in uniaxially strained (110)/110 bulk planar n-MOSFETs. Dashed: Piezoresistive model Solid+Symbs.: Simulations 50 Δμ/μ [%] 0 -2 [110] compr. stress 0 -2 -10 (110) Si closed: Experiments [17] open: Simulations 2 Δμ/μ [%] 0.1 4 closed: Experiments [24] open: Simulations 5 Δμ/μ [%] |k| [2π/a0] 0.2 200 0.0 VG-VT [V] 0.5 0 1.0 Figure 21: Inﬂuence of additional uniaxial εxx strain upon ID,Sat in FinFETs. Strain induced by epi-Si1−x Gex S/D for p-MOS and by wafer bending for n-MOS. ID,Sat is boosted by 13% for p-MOS with x=25% and by 21% for nMOS with 460MPa stress. Uniaxial strain boosters are thus effective in presence of large εzz .